View stunning SlideShares in full-screen with the new iOS app!Introducing SlideShare for AndroidExplore all your favorite topics in the SlideShare appGet the SlideShare app to Save for Later — even offline
View stunning SlideShares in full-screen with the new Android app!View stunning SlideShares in full-screen with the new iOS app!
4724 J. VAN WINGERDEN et al. 55
FIG. 2. Four different binding geometries (A-D) for ad-dimers.
different dimer conﬁgurations have been observed in these
experiments. The A and B dimers, which reside on top of the
dimer rows, are well known and easily identiﬁed by the di-
rection of their elongation see Figs. 3 a , b . The appear-
ance of the C and D dimers in STM images requires special
attention as they have not been described previously.
We have never observed isolated D dimers. This is in
accordance with the predictions based on ab initio
calculations.16 To show what an isolated D dimer might look
FIG. 1. Empty-state STM images with coverages of 0.012 ML like, we present in Figs. 3 c , d clusters that contain D
a , 0.05 ML b , 0.18 ML c , and 0.20 ML d . The layers have dimers. Nearly all D dimers we observe have a neighboring
been deposited in 10 min a , b , d or 15 min c . Tunneling con- B dimer see, e.g., dimer D 3 ). This corresponds to the DB
ditions: 0.4 nA, 1.3 V a – c ; 1.0 nA, 1.5 V d . structure required for the formation of an epitaxial overlayer.
Dimers D 1 and D 2 form a cluster together and show the
sition is also discussed. The analysis of the complete growth appearance of D dimers without a neighboring B dimer.
process has been based on a large number of images obtained Three examples of the structure that we have identiﬁed as
from samples with various coverages. The analysis covers the C dimer are shown in Figs. 3 a,b . While they are clearly
nearly all structures observed in the experiments. All other visible in the empty state image Fig. 3 b , their appearance
structures that have been observed did not seem to be rel- in the ﬁlled-state image Fig. 3 a is even fainter than that of
evant for the growth process, as they only occurred occasion- the substrate dimers. In comparison with the D dimers D 1
and D 2 Figs. 3 c , d , the structures C 1 -C 3 in Figs. 3 a ,
Experiments are performed in a UHV system with a base
pressure of 5 10 11 Torr. A commercial Beetle type STM20
with a Pt-Ir tip is used for measuring the constant current
STM images. Movies, made by capturing images at 10-s
time intervals, show the surface dynamics at room tempera-
ture. For all dynamic processes observed with the STM we
need to keep in mind that they may be inﬂuenced by the
electric ﬁeld. Nevertheless, they give useful indications for
possible pathways with a reasonable transition rate at or
slightly above room temperature, as was shown in a previous
study.21 Silicon 001 surfaces are prepared by ﬂashing to
1250 °C, yielding the (2 1) reconstructed surface with
monolayer height steps. Deposition at room temperature is
performed at least 4 h after ﬂashing the sample. As waiting
for a longer period does not change the results, the sample
temperature is close enough to room temperature. Silicon is
deposited from a commercial miniature electron-beam
III. ISOLATED AD-DIMERS FIG. 3. Filled-state image a showing an A dimer, a B dimer,
and three C dimers (C 1 -C 3 ) together with empty-state image b ,
The smallest immobile islands created during room- where the A dimer has rotated back to the B orientation. Filled- c
temperature growth on Si 001 are ad-dimers. For denoting and empty-state d images where three D dimers are indicated as
the different binding geometries of the most probable sites D 1 -D 3 . D 3 looks different because there is a B dimer on top of the
we use the notation shown in Fig. 2. We have been able to neighboring dimer row. Tunneling conditions: 0.4 nA a – d and
identify these dimer conﬁgurations in our STM images. No 1.3 V a , c ; 1.3 V b ; 1.15 V d .
55 ROOM-TEMPERATURE GROWTH OF SUBMONOLAYERS OF . . . 4725
FIG. 4. Filled- a , c and empty-state b , d images of C
dimers with perfect a , b and imperfect c , d buckling like a
circle of adatoms. Tunneling conditions: 1.5 nA, 1.3 V a ; 1.5 nA,
1.3 V b ; 1.1 nA, 1.3 V c ; 1.1 nA, 1.3 V d .
b have an aspect ratio much closer to unity. Nevertheless,
we observe that their long axis is directed perpendicular to
the dimer rows. Similar differences are observed between
B and A dimers. This supports the identiﬁcation of the struc-
ture as a dimer located in between the dimer rows with the
dimer bond parallel to the substrate dimer bonds, i.e., as a
C dimer. In the ﬁlled-state image Fig. 3 a the C dimers are FIG. 5. a Density of isolated A, B, and C dimers in arbitrary
characterized by a surrounding ‘‘circle’’ of visible substrate units as a function of coverage. Straight lines indicate the linear
atoms. The interaction between dimers along the substrate increase with coverage for the lower three coverages. b The per-
dimer rows causes an anticorrelated buckling which is vis- centage of isolated dimers in the C position as a function of cover-
ible over a range of about six dimers at both sides of the age. The line corresponds to a ratio of 2/3.
structure. In the ﬁlled-state images the C dimers appear in
different forms. Most C dimers do not exhibit a circle of percentage of isolated ad-dimers in the C positions matches
visible substrate atoms as perfect as that shown in Fig. 4 a . the exact value of 2/3 remarkably well. This strongly sug-
Instead, we often observe imperfect circles, where one or gests the following, kinetically determined origin for the dis-
two of the atoms forming the circle seem to be missing Fig. tribution. According to ab initio calculations12,13 the adatoms
4 c . The empty-state image in Fig. 4 d , however, shows will diffuse on top of the dimer rows, making frequent side
that they are still there. The exact origin of these imperfec- trips to the more stable sites at either side of the rows. Dif-
tions is not yet clear. fusion across the dimer rows is not activated at room tem-
From the STM images the abundances of the structures perature. Therefore, the adatoms remain on the dimer row on
have been determined for different coverages see Fig. 5 a . which they are deposited. We now assume that two adatoms
For low coverages i.e., less than one dimer per substrate separated by more than one dimer row cannot form a dimer
dimer row the numbers of isolated A, B, and C dimers and that the type of dimer formed only depends on the row
increase linearly with coverage. At a coverage of about 0.01 on which the second adatom is deposited. Then, dimers are
ML see Fig. 1 a the formation of multiple-dimer clusters formed either from two adatoms on neighboring dimer rows
reduces the rate of increase of the number of isolated ad- or from two adatoms on the same row. This results in a
dimers. A and B dimers have been observed to transform chance of 2:1 that the second adatom is deposited on a neigh-
into each other at room temperature.21,15,19 Hence, it is justi- boring row instead of on the same row. If the adatoms meet
ﬁed to assume that these populations are in thermodynamic on the same dimer row A/B dimers are formed. If they meet
equilibrium and, therefore, we will often address them as the on neighboring rows a C dimer is formed. This causes 2/3 of
A/B population. From the ratio B:A of 10:1 the energy dif- the dimers to be formed in the C position as observed ex-
ference of the sites can be estimated. This yields a 60-meV perimentally.
lower energy for the B site compared to the A site. This near This model for the dimer formation may seem to contra-
degeneracy of A and B dimers is in accordance with theo- dict the observations of Wolkow,14 who described the exclu-
retical calculations.16–19 sive formation of A/B dimers from adatoms on neighboring
Of all isolated ad-dimers 67% are in the C position see dimer rows at a temperature of 160 K. The apparent interac-
Fig. 5 b . If we assume that the C dimer population is in tion between adatoms on different rows was attributed to
thermodynamic equilibrium with the A/B population we ﬁnd strain effects. However, these subtle strain effects will be
an energy difference of only 20 meV between the C and washed out at room temperature. Consequently, at room tem-
A/B sites. This contradicts ab initio calculations17,18 that pre- perature other interactions dominate the formation of dimers.
dict an energy difference larger than 100 meV. There are, As discussed before the abundances of A/B and C dimers
however, a number of indications that the abundance of the are kinetically determined. Therefore, room-temperature de-
C dimers is kinetically determined. First of all, we did not posited submonolayers cannot reveal any information about
observe with our STM any switching of isolated ad-dimers the energy differences of these sites. Annealing experiments
between the C position and the A/B positions. Secondly, the may be performed to determine the thermodynamic stability
4726 J. VAN WINGERDEN et al. 55
FIG. 6. Filled- a and empty state b images of a three-atom
cluster with a schematic drawing c of a C dimer with the two
possible binding sites 1,2 for an adatom to form a stable three- FIG. 7. Empty-state images from a movie and schematic draw-
atom cluster. Tunneling conditions: 0.3 nA, 1.3 V a ; 0.3 nA, ings demonstrating the formation of a three-atom structure from a
1.3 V b . B dimer and an invisible extra adatom before a and after forma-
tion b . Subsequent rotation of dimer B 2 to the A conﬁguration c
enables comparison of an atomically resolved A dimer with a three-
of the isolated ad-dimers. For interpreting such experiments
atom structure. In b dimer B 3 from a and c is in the A con-
it has to be realized that the C dimers may still be frozen in
ﬁguration. Tunneling conditions: 0.4 nA, 1.7 V.
their positions while the diffusion of A/B dimers is already
activated and causes the formation of clusters. Annealing
experiments19 have been reported to result in an increase of however, is exactly the visible effect in ﬁlled-state images if
the number of dimers in between the substrate dimer rows. a C dimer catches an adatom, as can be seen from the com-
This observation is, however, probably due to the formation parison of the C dimer appearances in Figs. 4 a and 6 a .
of tetramers, which are easily misinterpreted as isolated A more surprising observation is the existence of a second
dimers.21 pathway for the formation of the three-atom cluster. Here, an
A/B dimer is converted into a three-atom cluster. In this case
the transition is more complex because the dimer bond of the
IV. THREE-ATOM CLUSTERS
A/B dimer is broken during the transition. The three images
As ad-dimers are immobile at room temperature, stable in Fig. 7 showing this conversion are obtained from an STM
nuclei can only grow by the addition of adatoms. The ﬁrst movie. In Fig. 7 a we observe three B dimers on one dimer
step in this growth process is the formation of a three-atom row. One of these B dimers (B 1 ) catches an extra adatom
cluster by adding one adatom to an ad-dimer. We only ob- and forms a three-atom cluster as shown in Fig. 7 b . That
served one type of stable three-atom cluster, an example of this structure is indeed a three-atom structure is conﬁrmed by
which is shown in Figs. 6 a , b . In this cluster an atom is Fig. 7 c . In contrast to the A dimer, the three-atom structure
bound next to a C dimer at site 1 or 2 in the schematic exhibits one elongated spot and one spot that is similar to
drawing in Fig. 6 c . In this manner all three atoms are po- those of the A dimer. The elongated spot originates from the
sitioned on one line perpendicular to the substrate dimer C dimer and its midpoint is visibly shifted towards the
rows. Our observation that this is the only stable three-atom middle of the trough between the substrate dimer rows.
cluster is corroborated by the work of Yamasaki, Uda, and Both conversion processes starting from A/B or C dimers
Terakura,18 who did not ﬁnd other stable three-atom clusters occur with more or less equal probability. Forming three-
in their calculations. In ﬁlled-state images the C dimer of the atom clusters exclusively from either C or A/B dimers
three-atom structure is now also visible as a bright spot in would change the ratio of their abundances of 2:1. For a
contrast to its appearance as an isolated ad-dimer. The ada- coverage of about 0.012 ML, where 15% of the atoms have
tom of this structure is invisible in the ﬁlled-state images. formed a three-atom cluster, the abundance of isolated ad-
This adatom is indicated with an asterisk in the empty-state dimers in the C position is still 2/3. Using only the C dimer
image, Fig. 6 b . for forming three-atom clusters would have caused a small
The most straightforward mechanism for the formation of but signiﬁcant decrease of the C dimer abundance from
a three-atom cluster is the sticking of an adatom to a C 67% to 63% . The absence of any change in the ratio of the
dimer. This adatom can arrive at either side of a C dimer via abundances indicates roughly equal efﬁciencies for forming
diffusion along the dimer rows next to the C dimer. Experi- three-atom clusters by sticking adatoms to either C or A/B
mental evidence for this pathway is the fact that we observed dimers. This also suggests that A/B dimers cannot be trans-
several C dimers in ﬁlled-state images turning bright. Be- formed into three-atom clusters by atoms diffusing on the
cause we do not have empty-state images of these transi- same dimer row. In that case the capture area for atoms
tions, the addition of the extra atom has not been observed causing the transformation only comprises the two neighbor-
directly. The observed increase in brightness of the C dimer, ing dimer rows for both A/B and C dimers. This assumption
55 ROOM-TEMPERATURE GROWTH OF SUBMONOLAYERS OF . . . 4727
is conﬁrmed by ab initio calculations,18 as these calculations
did not yield any evidence for interactions between adatoms
and A/B dimers on the same dimer row.
V. DILUTED DIMER ROWS
The three-atom clusters described in the preceding section
act as templates for forming larger nonepitaxial structures.
They are extended by sticking adatoms in line with the atoms
of the cluster at either end of the structure. If adatoms are
bound at both sides of a C dimer sites 1 and 2 in Fig. 6 c ,
a four-atom cluster is formed. In a previous study21 we have
demonstrated that this structure, which we called a ‘‘cross
structure,’’ is formed from two dimers on neighboring sub-
strate dimer rows. In our present study we also observed the
cross structure. Because the submonolayers in this study are
grown at room temperature, where ad-dimers are immobile, FIG. 8. A V-shaped row of C dimers in the 310 directions;
we conclude that the cross structure can also be built up atom ﬁlled state a and empty state b . The four metastable binding sites
by atom. The general form of the structure obtained by ex- 1 – 4 for adatoms involved in the formation of 310 lines are
tending the three-atom cluster with an arbitrary number of schematically depicted in c . Tunneling conditions: 0.4 nA, 1.3 V
a ; 0.4 nA, 1.3 V b .
atoms is a line of atoms along the 110 direction, i.e., per-
pendicular to the substrate dimer rows. This 110 line con-
can be formed with an atom diffusing on the same dimer
sists of a number of C dimers in neighboring troughs be-
row. An atom diffusing on the neighboring dimer row will
tween the substrate dimer rows. Either end of the 110 line
yield a new C dimer and extend the row along the 310
can consist of a C dimer or an adatom. These structures have
been described before9,21,15 and are denoted as diluted dimer
We have no direct evidence for the existence of the pre-
rows. The process governing their formation is analogous to
cursor state, but we have observed ‘‘clusters’’ of precursor
the surface polymerization reaction described for Al on
states, an example of which is shown in Fig. 9. We expect
Si 100 .22
that the adatom binding sites of the precursor state are not
A puzzling question is the difference in brightness be-
stable at room temperature, but that they have nevertheless
tween isolated C dimers and C dimers in these diluted dimer
an increased occupancy during the growth. The combination
rows. We propose two explanations, based on the geometries
of two precursor states shown in Fig. 9 does become stable at
of the two structures obtained from ab initio calculations.17
First, the dimer bond for the C dimer in the row is much
The C dimers in the 310 chains are only faintly visible
shorter than that of the isolated dimer. We expect the result-
in the ﬁlled-state images, as in the case of isolated C dimers.
ing increased overlap of the atomic orbitals to lead to a
higher density of states above the dimer, and hence to a Therefore, the neighboring C dimers in these lines do not
brighter appearance in the STM images. Second, the dimer in seem to inﬂuence the C dimer bonds as strongly as in the
the row is buckled, whereas the isolated one is symmetric. case of the diluted dimer rows.
Naturally, the upwards buckled atom appears higher than We can now describe the growth up to doses of about 0.2
that of a symmetric dimer. This effect can even be enhanced ML. At very low doses ( 0.05 ML we get the structures
by a charge transfer from the downwards buckled atom to the described in Secs. III and IV. When growth proceeds further,
upwards buckled atom. The dimer appears symmetric in the adatoms stick to existing structures, forming one of the linear
image due to temperature activated switching. structures described in Secs. V and VI. Other structures are
relatively rare. Because extension of the linear structures oc-
curs either in the 110 or in the 310 direction, we end up
VI. DIMER ROWS ALONG †310‡ DIRECTIONS with a kind of random network of atomic line segments in
Apart from the known diluted dimer rows we observed a
linear structure that also consists of C dimers. The structure
is formed along 310 and its symmetry related directions. It
is very common at doses above 0.05 ML. A special V-shaped
example consisting of two connected linear segments is
shown in Figs. 8 a , b .
The formation of the rows along the 310 directions can
be explained if we assume a precursor state in which an
adatom is bound near a C dimer in one of the four metastable
binding sites 1-4 in Fig. 8 c . These sites may originate
from the strain induced by the presence of the C dimer. The
interaction of adatoms bound at these sites with other diffus- FIG. 9. Filled- a and empty-state b images with a schematic
ing adatoms will lead to the formation of new dimers. Analo- drawing inset in a of a cluster of two three-atom precursor states.
gous to the formation of isolated ad-dimers an A/B dimer Tunneling conditions: 0.4 nA, 1.3 V a ; 0.4 nA, 1.3 V b .
4728 J. VAN WINGERDEN et al. 55
FIG. 10. Diluted dimer row ending with BD epitaxial segment
a and one ending with a twin b . The straight lines in a are FIG. 11. Pathway for the conversion of diluted dimer row ends
plotted to indicate the edges of a substrate dimer row, which can be a into epitaxial segments d . A three-atom cluster e is converted
deduced from the position of the vacancy in this row at the lower into a cross structure f by the addition of an extra adatom. This
right end. Tunneling conditions: 0.4 nA, 1.3 V. structure can transform into a twin structure g .
these directions, with relatively open areas in between them the conversion process are not too large. At present we do
see Fig. 1 c . At this stage of the growth deposited atoms not have a sequence of consecutive images showing the com-
are rapidly captured by one of the numerous metastable plete conversion process. However, we did observe all the
binding sites of the network. individual steps.
The formation of a B dimer at the end of a diluted dimer
VII. TRANSITION TO EPITAXIAL STRUCTURES row according to the ﬁrst step in the conversion path from
a to b in Fig. 11 has been observed earlier,21 but in these
After deposition of nearly 0.2 ML the majority of the observations the transition activity was clearly enhanced by
deposited material still occupies nonepitaxial binding sites, the presence of the electric ﬁeld. The proposed conversion
since most of the ad-dimers in the network are in the C path requires the consecutive occurrence of two of these
position. Further growth now causes a conversion of the ma- transitions to form a twin structure at the end of the diluted
jority of nonepitaxial diluted dimer rows into epitaxial dimer dimer row. This may reduce the conversion rate. However,
rows. At 0.18-ML coverage see Fig. 1 c already a few the fact that we have observed a few diluted dimer rows
diluted dimer rows are observed to be partially converted ending with a twin structure see Fig. 10 b proves that the
into epitaxial dimer rows. A pronounced increase in the ﬁrst two steps of the conversion path see Figs. 11 a –11 c
abundance of epitaxial structures is obvious from the com- do exist. Furthermore, we have observed that about 4% of
parison of Fig. 1 c and Fig. 1 d , which originate from dif- the atoms form twin structures at 0.18 ML coverage. This
ferent experiments. The abundance of epitaxial structures demonstrates that under growth conditions the conversion to
with at least 4 atoms increases from 38 to 50% while the twin structures does occur at a reasonable rate. These twins
dose differs only 0.02 ML. The fact that a substantial con- can only be formed from a diluted dimer row, i.e. in a pro-
version to epitaxial structures does not take place at an ear- cess similar to the ﬁrst two steps of the conversion path,
lier stage of growth indicates that there exists a considerable which is concluded from the following reasoning. Growth is
barrier for this transition. performed at room temperature and, therefore, occurs exclu-
We observed the following characteristics of the partially sively by the addition of single adatoms. This means that the
converted diluted dimer rows: 1 apart from a few excep- precursor for the twin structure with four atoms should be a
tions, where diluted dimer rows contain a single epitaxially three-atom structure. Because we only observed three-atom
oriented dimer, the smallest epitaxial segments always con- structures with a C dimer, the most likely pathway see Figs.
tain two dimers; 2 the conversion occurs exclusively at the 11 e –11 g is the formation of a cross structure a diluted
ends of the diluted dimer rows; 3 epitaxial segments with dimer row with four atoms , which is then converted to a
the outer dimer being a B or D dimer are both observed. An twin structure. The latter process is identical to the ﬁrst part
example of one ending with a D dimer is presented in Fig. of the conversion to an epitaxial segment.
10 a . Once a twin structure has been formed, an epitaxial seg-
A pathway accounting for the above-mentioned experi- ment is formed compare Figs. 11 c , d by a collapse to a
mental observations is depicted in Fig. 11. It initiates by BD structure as shown in the STM images in Fig. 12. The
forming a B dimer from an atom of the outer C dimer with two B dimers of one of the twins in Fig. 12 a are indicated
the adatom at the end of the diluted dimer row. This process with arrows. After the collapse see Fig. 12 b the distance
has been observed with STM previously.21 Repeating the of the dimers has been halved, in accordance with the for-
process at the end of the remaining diluted dimer row then mation of the BD epitaxial segment. Similar epitaxial struc-
creates a modiﬁed BB structure, which we previously de- tures with two dimers are frequently observed on room-
noted as a ‘‘twin.’’21 Finally, a collapse of this twin structure temperature-grown submonolayers. This shows the existence
leads to an epitaxial BD segment. This conversion path of the transition under growth conditions. The transition of
yields a sequence ending with: C, adatom, B, D. the twin structure to the BD cluster has recently been studied
The conversion path is fairly complex and the major ques- with ab initio methods.18 The transition mechanism explored
tion is whether the kinetic barriers for the steps involved in in these calculations has an activation energy of 1.6 eV. This
55 ROOM-TEMPERATURE GROWTH OF SUBMONOLAYERS OF . . . 4729
FIG. 12. Sequence of transitions from an STM movie, showing
the formation of an epitaxial structure b from a twin a . Dimers
of the twin and the epitaxial structure are indicated with arrows.
The extra adatom indicated with an asterisk from a neighboring
structure is attached to the epitaxial segment in c . Tunneling con-
ditions: 0.4 nA, 1.6 V.
activation energy renders the transition mechanism practi-
cally forbidden at room-temperature, while we do observe
BD clusters after room-temperature growth. Apparently, FIG. 13. Overview of the evolution of the relevant structures
there should exist an alternative conversion mechanism with during room temperature growth of silicon on Si 001 .
a lower activation barrier.
The proposed conversion path accounts for the formation
of epitaxial segments ending with a D dimer, which is ob- lution of the relevant structures during growth is schemati-
served to be the case for at least 50% of the observed seg- cally depicted in Fig. 13. The growth starts with adatoms
ments. It does not explain the form of the other epitaxial forming ad-dimers. We found that adatoms diffusing on the
same dimer row form A or B dimers, while adatoms on
segments, which end with a B dimer. These segments may
neighboring dimer rows yield C dimers. Stable three-atom
be formed along the path proposed by Brocks and Kelly.17
clusters with all atoms aligned along one row perpendicular
This conversion path initiates with the arrival of an adatom
to the substrate dimer rows can be formed if adatoms stick to
and always results in a segment ending with a B dimer.
A, B, or C dimers. These stable three-atom clusters form the
The conversion path for the formation of epitaxial seg-
precursor state for the lines of dimers along the 110 direc-
ments is expected to be very sensitive to the local geometry.
tion diluted dimer rows . Apart from the diluted dimer rows,
Local modiﬁcations of the strain distribution induced by
lines of dimers can also be formed along the 310 and its
neighboring structures may facilitate the occurrence of the
symmetry related directions. The three-atom precursor state
complex transitions to epitaxial structures at higher cover-
for these lines is probably the one depicted in Fig. 13. Its
ages. This explains the rapid increase of the abundance of
adatom binding site, however, is not as stable as that in the
epitaxial structures at about 0.2 ML. Further investigations
three-atom cluster which has all atoms in one line. Both the
are needed to quantify these local strain effects.
110 dimer lines and the 310 lines are compatible with
We often observe single adatoms bound at the end of
each other in the sense that structures consisting of con-
epitaxial segments but they are not a clue for the conversion
nected segments of both line types can be formed. Finally, a
process as they do not necessarily originate from the conver-
transition to epitaxial structures occurs by the formation of
sion process. This is demonstrated in the transition that oc-
epitaxial segments in diluted dimer rows. Based on STM
curred between Figs. 12 b and 12 c . Here, an adatom
observations a possible pathway for this conversion process
bound nearby has moved and is ﬁnally bound alongside the
is proposed. The shortest diluted dimer row that can be con-
D dimer of the epitaxial structure. Epitaxial segments both
verted to an epitaxial structure consists of a C dimer with
with and without an extra adatom have been observed. As
two atoms cross structure . Its conversion into an epitaxial
the transition in Fig. 12 shows, the extra adatoms can origi-
structure occurs via the twin modiﬁed BB cluster as shown
nate from nearby structures. Furthermore, atoms deposited
in Fig. 13.
afterwards may also bind at these sites.
Thus we have shown that epitaxial structures are formed
during deposition of submonolayers of silicon on Si 001 .
VIII. CONCLUSIONS For growing thicker layers the probability for adatoms to
The evolution of structures during room-temperature step down at the step edges further inﬂuences the epitaxial
deposition of submonolayers of silicon on Si 001 has been quality. The room-temperature activation of that process re-
presented. The data are obtained by a careful analysis of all quires a separate study.
features observed in numerous STM images of the Si 001 ACKNOWLEDGMENTS
surface after deposition of different coverages. All observed
features have been described except for the defects and those We thank G. Brocks for helpful discussions. Furthermore,
structures that occur in such small numbers that they do not the technical support of C.D. Laman, R.F. Staakman, and H.
seem to be of importance for the growth process. The evo- Vogelaar is gratefully acknowledged.
4730 J. VAN WINGERDEN et al. 55
D.J. Eaglesham, H.-J. Gossmann, and M. Cerullo, Phys. Rev. B.S. Swartzentruber, Phys. Rev. Lett. 76, 459 1996 .
Lett. 65, 1227 1990 . G. Brocks, P.J. Kelly, and R. Car, Phys. Rev. Lett. 66, 1729
J.M. Gibson, H.-J. Gossmann, J.C. Bean, R.T. Tung, and L.C. 1991 .
Feldmann, Phys. Rev. Lett. 56, 355 1986 . 13
Q.-M Zhang, C. Roland, P. Boguslawski, and J. Bernholc, Phys.
H.-J. Gossmann and L.C. Feldmann, Phys. Rev. B 32, 6 1985 . Rev. Lett 75, 101 1995 .
H.-J. Gossmann and L.C. Feldmann, Appl. Phys. A 38, 171 14
R.A. Wolkow, Phys. Rev. Lett. 74, 4448 1995 .
1985 . 15
P.J. Bedrossian, Phys. Rev. Lett. 74, 3648 1995 .
F. Jona, Appl. Phys. Lett. 9, 235 1966 . 16
G. Brocks, P.J. Kelly, and R. Car, Surf. Sci. 269-270, 860 1992 .
T. de Jong, W.A.S. Douma, L. Smit, V.V. Korablev, and F.W. 17
G. Brocks and P.J. Kelly, Phys. Rev. Lett. 76, 2362 1996 .
Saris, J. Vac. Sci. Technol. B 1, 888 1983 . 18
T. Yamasaki, T. Uda and K. Terakura, Phys. Rev. Lett. 76, 2949
A.V. Zotov, S.V. Ryzhkov, and V.G. Lifshits, Surf. Sci. 328, 95
1995 . 19
8 Z. Zhang, F. Wu, H.J.W. Zandvliet, B. Poelsema, H. Metiu, and
Y.-W. Mo, B.S. Swartzentruber, R. Kariotis, M.B. Webb, and
M.G. Lagally, Phys. Rev. Lett. 74, 3644 1995 .
M.G. Lagally, Phys. Rev. Lett. 63, 2393 1989 . 20
9 K. Besocke, Surf. Sci. 181, 145 1987 .
Y.-W. Mo, R. Kariotis, B.S. Swartzentruber, M.B. Webb, and 21
A. van Dam, J. van Wingerden, M.J. Haye, P.M.L.O. Scholte, and
M.G. Lagally, J. Vac. Sci. Technol. A 8, 201 1990 .
D. Dijkkamp, E.J. van Loenen, and H.B. Elswijk, in Ordering at F. Tuinstra, Phys. Rev. B 54, 1557 1996 .
Surfaces and Interfaces, edited by A. Yoshimori, T. Shinjo, and G. Brocks, P.J. Kelly, and R. Car, Phys. Rev. Lett. 70, 2786
H. Watanabe, Springer Series in Materials Science Vol. 17 1993 .
Springer, Berlin, 1992 .